WARM MIX ASPHALTS WITH CECABASE RT ADDITIVE: PROPERTIES AND ADVANTAGES
J. González-León, V. Luca
Centre de Recherche Rhône-Alpes ARKEMA, Rue Henri Moissan, B.P. 63 Pierre-Bénite, France 69493
[email protected] ABSTRACT Recently, new technologies have been developed to reduce the environmental impact of the road construction industry. Among them, the technologies that allow a substantial reduction on the energy consumed during the production of hot asphalt mixtures have taken a very important role. There are several technologies, based on very different physicochemical phenomena that allow producing what is now known as warm mix asphalts. The work presented here describes the use of one particular type of warm mix asphalt technology based on chemical additives. This technology has been already proven to work under very different laboratory and field job conditions. It is based on the use of surfactant-type additives that enhances the workability of an asphalt mix allowing it to be paved and compacted at lower temperatures. Only a low concentration, from 0.2 to 0.5wt% with respect of bitumen, is required to have the desired effect. The several advantages observed by the use of this warm mix asphalt technology are presented in this work, including field job examples, measured energy consumption reductions and environmental measurements. It is also a matter of this work the discussion of the enhanced functionality that this particular kind of additives may provide. Examples of such are their role as adhesion promoters in the asphalt mixture and as aids on the incorporation of higher amounts of reclaimed asphalt pavement.
1. INTRODUCTION – WARM MIX APSHALTS
The term warm mix asphalts (WMA) has been given to those asphalt mixtures that are produced and paved at lower temperatures to those normally used in standard hot mix asphalts (HMA). During the last years, there has been an important development on the different technologies that allow such reduction of temperature and on the characterization of the resulting pavements. Currently, there are more than 20 different technologies that allow the production of WMA . These techniques actually depend on very different physical and chemical processes to allow the production of WMA. The main challenge is to enhance the workability of the asphalt mixture as the temperature is reduced. As the temperature is reduced, the bitumen increases its viscosity making the covering of the aggregates and the compaction of the mix more difficult . The several WMA technologies on the market can nevertheless been grouped on four categories, based on the physical principle used for enhancing the workability of the mixture at reduced temperatures: Sequencing of hard and soft bitumens – One of the first technologies developed for WMA production was the one developed by Kolo Veidekke . In this technique, sequential mixing of a portion of the aggregates with a hard bitumen is done before the rest is mixed with a foamed softer bitumen. This approach requires a substantial modification of the production plant (as it is actually a different process) and handling of different binders. Water foam processes – This is a large group that includes probably the majority of WMA technologies on the market. In all of them, bitumen foam is produced by evaporation of water during the mixing process. The water vapour produced when in contact with the hot bitumen increases the surface area of the binder as well as provides additional energy to the system to better cover the aggregates. It is claimed by some technology providers that the amount of residual water (in liquid or vapour form) is key to maintain the workability of the mix afterwards. The main difference between the technologies in this group is the way the water and the binder contact takes place. One option is to add mineral additives that contain water to be released only at higher temperatures (as those used for asphalt mix production), an example of such additives are the zeolithes [3,4]. A different option is to produce the foam at the same time the bitumen is injected into the mixer. Such technologies are based on the actual machine (nozzle system) that can effectively generate the foam at such point of the mix production . Another option is to only partially dry a portion of the mineral formula before adding the binder . Such approach has the potential to reduce even further the temperature of production (as it may be below 100°C). However, the control of the amount of water present of the aggregate fraction, being key to the process, may be challenging. On last example of the foaming approach is to actually use a bitumen emulsion, instead of a dry binder. In this case the water is already in close contact to the bitumen when in contact with the heated aggregate . Waxes – In this case, an additive is added into the bitumen to reduce its viscosity at mixing temperatures only. This has been achieved through the use of waxes [3,4]. The waxes are chosen such that they melt above about 100-110°C. On the melt state, they can decrease the viscosity of the bitumen, improving the bitumen covering of the aggregates and the workability of the mixture. At lower temperatures, they crystallize, reinforcing the bitumen at application conditions. They are usually used at concentrations of about 2 to 3% by weight of the binder. Care should be taken, not to work at temperatures lower than the crystallization temperature of the wax. These additives do modify the properties of the
bitumen, in particularly the low temperature properties , and could actually change its grade. Chemical additives – On this group we found additives that act on a very different way than the before-mentioned wax additives. Contrary to waxes that modify the bulk of binder, the chemical additives act only at the interface between the mineral aggregate and the bitumen . This is the reason why these additives actually are used on very small doses (from 0.3% to 0.6% by weight with respect of binder). The reported benefits of WMA had been also subject to several previous publications [1,3,9]. There are several benefits as a consequence of reducing the temperature of an asphalt mix production. These advantages are mainly the reduction on energy used in the production and the reduction of the emissions related to this reduction in temperature. Other advantages such as the comfort to the workers can also be cited. However, some advantages are unique to each technology since they are the results of the particular mechanisms to achieve the reduction in temperature In this work, a further discussion about the chemical additives is done. The properties of the asphalt binder comprising the additives as well as on the asphalt mixture are presented. The observed advantages by the use of the chemical additives, both those related to the reduction in temperature as well as those unique to the chemical additives are presented. The laboratory work and field jobs described and discussed in this work were carried out using a commercial additive patented by CECA, named CECABASE RT. These are liquid additives, which used at 0.3% to 0.5% by weight of the bitumen, are claimed to allow a reduction in asphalt mix production temperature of about 40°C . More than 2.5 million tons of asphalt mix have already been produced around the world with these additives.
2. HOW CHEMICAL ADDITIVES WORK
The chemicals used for the production of WMA are actually surfactant-like molecules. As any surfactant molecule, they are capable of changing the interfacial interactions between two different phases. In this case the chemical additives interact at the mineral and bitumen interphase, changing the way the mineral interact between each other. A smaller amount of additive is required to cover the surface of the mineral aggregates than to actually change the properties of the whole volume of bitumen. This is the reason why such a small amount of chemical additive, between 0.3% and 0.6%, is required to produce WMA. At this small concentration of additive, even if it is a liquid with a lower viscosity than hot bitumen, the properties of the bitumen remain mainly unchanged. The viscosity and mechanical properties of the bitumen containing a chemical additive for WMA are not modified by its presence. The viscosity as a function of temperature of a bitumen with and without a chemical additive for WMA was measured. A dynamical shear rheometer with temperature controlling capabilities was used to measure the viscosity at a shear rate of 100/s under a parallel-plate geometry. Figure 1a shows the viscosity curve of bitumen with a penetration grade of 35/50 1/10mm containing 0.3% of Cecabase RT additive. On the same curve, the viscosity of the original bitumen without the additive is also shown. It can be seen that the two curves are almost identical at the measured temperatures. Another measurement was carried out at lower temperatures to evaluate the effect of additives at normal use temperatures. The parameter G*/sin δ was measured using the same rheometer at a frequency of 2 Hz and 1% strain as a function of temperature between 20 and 100°C.
Figure 1b shows the curves of the 35/50 1/10mm bitumen with and without the chemical additive. It can be seen that the two curves superpose each other, demonstrating that there is practically no change on the bitumen rheological properties under the conditions of the test. If the high temperature performance grade criteria (PG–grade) is use
Click here to load reader